#------------------------------------------------------------------------------
#$Date: 2023-12-22 17:07:40 +0200 (Fri, 22 Dec 2023) $
#$Revision: 288505 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/33/55/4335585.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4335585
loop_
_publ_author_name
'Olena V. Sharga'
'Andrey B. Lysenko'
'Marcel Handke'
'Harald Krautscheid'
'Eduard B. Rusanov'
'Alexander N. Chernega'
'Karl W. Krämer'
'Shi-Xia Liu'
'Silvio Decurtins'
'Adam Bridgeman'
'Konstantin V. Domasevitch'
_publ_contact_author_address
;         
        Inorganic Chemistry Department
        Kiev Shevchenko University
        Volodimirska Str. 64
        01033 Kiev
        Ukraine
;
_publ_contact_author_email       ab_lysenko@univ.kiev.ua
_publ_contact_author_fax         +380(44)239-3306
_publ_contact_author_name        'Dr Andrey B. Lysenko'
_publ_section_title
;
 Unprecedented Trapping of Difluorooctamolybdate Anions within an
 α-Polonium Type Coordination Network
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              8784
_journal_page_last               8794
_journal_paper_doi               10.1021/ic400954x
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'C21 H40 Co3 F2 Mo8 N18 O31'
_chemical_formula_weight         2023.02
_chemical_name_systematic
;
tris[1,3-bis(1,2,4-triazol-4-yl)propane]-diaqua-difluorooctamolybdato
-tricobalt(II) Trihydrate
;
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                96.9040(10)
_cell_angle_beta                 94.8820(10)
_cell_angle_gamma                94.1450(10)
_cell_formula_units_Z            2
_cell_length_a                   12.6171(2)
_cell_length_b                   13.5719(3)
_cell_length_c                   14.8734(3)
_cell_measurement_reflns_used    9054
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      30.45
_cell_measurement_theta_min      2.16
_cell_volume                     2510.47(9)
_computing_cell_refinement       'SMART-NT (Bruker, 1998)'
_computing_data_collection       'SMART-NT (Bruker, 1998)'
_computing_data_reduction        'SMART-NT (Bruker, 1998)'
_computing_molecular_graphics    'Diamond 2.1e (Brandenburg, 1999)'
_computing_publication_material  'WinGX 1.70.01 (Farrugia, 1999)'
_computing_structure_refinement  'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.980
_diffrn_measured_fraction_theta_max 0.980
_diffrn_measurement_device_type  'Bruker APEXII area-detector diffractometer'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0333
_diffrn_reflns_av_sigmaI/netI    0.0403
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            40824
_diffrn_reflns_theta_full        30.45
_diffrn_reflns_theta_max         30.45
_diffrn_reflns_theta_min         1.39
_diffrn_standards_decay_%        0
_exptl_absorpt_coefficient_mu    3.008
_exptl_absorpt_correction_T_max  0.6611
_exptl_absorpt_correction_T_min  0.5201
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    2.676
_exptl_crystal_description       prism
_exptl_crystal_F_000             1950
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.15
_refine_diff_density_max         1.390
_refine_diff_density_min         -1.710
_refine_diff_density_rms         0.165
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.075
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     751
_refine_ls_number_reflns         14950
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.075
_refine_ls_R_factor_all          0.0379
_refine_ls_R_factor_gt           0.0304
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0188P)²+6.9735P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0668
_refine_ls_wR_factor_ref         0.0693
_reflns_number_gt                12845
_reflns_number_total             14950
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic400954x_si_001_3.cif
_cod_data_source_block           (3)
_cod_depositor_comments
;
The following automatic conversions were performed:
data name '_publ_contact_autor_name' replaced with
'_publ_contact_author_name' as specified in the replacement file
'/home/antanas/src/cod-tools/trunk/data/replacement-values/replacement_tags.lst'.

Automatic conversion script
Id: cif_correct_tags 4998 2017-03-02 13:24:31Z antanas 

The following automatic conversions were performed:

data name '_iucr_refine_instruction_details' was replaced with
'_iucr_refine_instructions_details' as specified in the replacement
file 'data/replacement-values/replacement_tags.lst'.

Automatic conversion script
Id: cif_correct_tags 9268 2022-04-12 08:56:07Z antanas 
;
_cod_database_code               4335585
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Co1 Co 0.5000 0.5000 0.0000 0.00755(11) Uani 1 2 d S
Co2 Co 0.40780(3) 0.28586(3) 0.12768(3) 0.00777(8) Uani 1 1 d .
Co3 Co 0.0000 0.0000 0.5000 0.00730(11) Uani 1 2 d S
Co4 Co 0.22761(3) 0.05470(3) 0.35661(3) 0.00755(8) Uani 1 1 d .
Mo1 Mo 0.40672(2) 0.28123(2) 0.383327(18) 0.00812(5) Uani 1 1 d .
Mo2 Mo 0.51875(2) 0.56532(2) 0.408418(18) 0.00711(5) Uani 1 1 d .
Mo3 Mo 0.38091(2) 0.75041(2) 0.47700(2) 0.01960(7) Uani 1 1 d .
Mo4 Mo 0.27290(2) 0.47507(2) 0.434798(19) 0.01020(6) Uani 1 1 d .
Mo5 Mo 0.16567(2) 0.11459(2) 0.120325(18) 0.00743(5) Uani 1 1 d .
Mo6 Mo -0.09308(2) -0.00215(2) 0.082874(18) 0.00753(5) Uani 1 1 d .
Mo7 Mo -0.26069(2) 0.14283(2) -0.019595(19) 0.01056(6) Uani 1 1 d .
Mo8 Mo -0.02501(2) 0.24641(2) 0.050974(19) 0.00975(6) Uani 1 1 d .
N1 N 0.3549(2) 0.4884(2) 0.06544(19) 0.0109(5) Uani 1 1 d .
N2 N 0.3236(2) 0.4081(2) 0.10909(19) 0.0099(5) Uani 1 1 d .
N3 N 0.1958(2) 0.5082(2) 0.10898(19) 0.0112(5) Uani 1 1 d .
N4 N 0.0337(2) 0.9092(2) 0.38151(19) 0.0102(5) Uani 1 1 d .
N5 N 0.1140(2) 0.9322(2) 0.32862(19) 0.0113(5) Uani 1 1 d .
N6 N 0.0373(2) 0.7861(2) 0.27263(19) 0.0116(5) Uani 1 1 d .
N7 N 0.4721(2) 0.3491(2) 0.94450(19) 0.0098(5) Uani 1 1 d .
N8 N 0.4355(2) 0.2722(2) 0.98980(19) 0.0108(5) Uani 1 1 d .
N9 N 0.4413(2) 0.2142(2) 0.84724(18) 0.0109(5) Uani 1 1 d .
N10 N 0.1640(2) 0.0054(2) 0.54706(19) 0.0102(5) Uani 1 1 d .
N11 N 0.2429(2) 0.0340(2) 0.49442(19) 0.0101(5) Uani 1 1 d .
N12 N 0.3198(2) -0.0033(2) 0.62111(18) 0.0094(5) Uani 1 1 d .
N13 N 0.5863(2) 0.4508(2) 0.11651(19) 0.0110(5) Uani 1 1 d .
N14 N 0.5504(2) 0.3739(2) 0.16174(19) 0.0103(5) Uani 1 1 d .
N15 N 0.7102(2) 0.4294(2) 0.22276(19) 0.0104(5) Uani 1 1 d .
N16 N 1.0266(2) 0.1323(2) 0.43559(19) 0.0102(5) Uani 1 1 d .
N17 N 1.1078(2) 0.1489(2) 0.38065(19) 0.0093(5) Uani 1 1 d .
N18 N 1.0029(2) 0.2693(2) 0.3761(2) 0.0119(5) Uani 1 1 d .
O1 O 0.4822(2) 0.1484(2) 0.13614(19) 0.0226(6) Uani 1 1 d .
O2 O 0.34213(18) -0.04698(18) 0.31331(17) 0.0131(5) Uani 1 1 d .
H2B H 0.3349 -0.0612 0.2558 0.020 Uiso 1 1 d R
H2A H 0.3339 -0.1005 0.3372 0.020 Uiso 1 1 d R
O3 O 0.35464(18) 0.16032(17) 0.38852(16) 0.0109(4) Uani 1 1 d .
O4 O 0.38535(18) 0.29436(18) 0.26869(15) 0.0118(5) Uani 1 1 d .
O5 O 0.4876(2) 0.56858(19) 0.29564(16) 0.0154(5) Uani 1 1 d .
O6 O 0.26075(19) 0.7705(2) 0.51596(19) 0.0196(5) Uani 1 1 d .
O7A O 0.3535(2) 0.75831(18) 0.35553(16) 0.0211(5) Uani 0.50 1 d P
F1A F 0.3535(2) 0.75831(18) 0.35553(16) 0.0211(5) Uani 0.50 1 d P
O8 O 0.2294(2) 0.47714(19) 0.32362(17) 0.0175(5) Uani 1 1 d .
O9 O 0.16153(19) 0.5002(2) 0.49096(18) 0.0184(5) Uani 1 1 d .
O10 O 0.64929(18) 0.52958(18) 0.41564(16) 0.0122(5) Uani 1 1 d .
O11 O 0.44890(17) 0.73092(17) 0.60539(15) 0.0102(4) Uani 1 1 d .
O12 O 0.54033(18) 0.69923(17) 0.45942(16) 0.0109(4) Uani 1 1 d .
O13 O 0.36207(18) 0.60103(17) 0.45189(16) 0.0105(4) Uani 1 1 d .
O14 O 0.44327(17) 0.44065(16) 0.42801(15) 0.0083(4) Uani 1 1 d .
O15 O 0.27777(17) 0.33578(17) 0.43193(16) 0.0109(4) Uani 1 1 d .
O16 O 0.26639(18) 0.19393(17) 0.08920(16) 0.0125(5) Uani 1 1 d .
O17 O 0.22065(18) 0.08871(17) 0.22497(16) 0.0115(4) Uani 1 1 d .
O18 O -0.17985(19) -0.07165(18) 0.13644(17) 0.0151(5) Uani 1 1 d .
O19 O -0.3136(2) 0.2458(2) 0.02924(19) 0.0218(6) Uani 1 1 d .
O20 O -0.3264(2) 0.1170(2) -0.12701(18) 0.0189(5) Uani 1 1 d .
O21 O 0.0662(2) 0.30948(19) -0.00503(17) 0.0172(5) Uani 1 1 d .
O22 O -0.0843(2) 0.33996(19) 0.11002(17) 0.0173(5) Uani 1 1 d .
O23 O 0.18710(18) -0.00186(17) 0.04261(16) 0.0109(4) Uani 1 1 d .
O24 O 0.07146(18) 0.21475(17) 0.15135(16) 0.0115(4) Uani 1 1 d .
O25 O 0.04163(17) 0.09980(17) 0.00707(15) 0.0093(4) Uani 1 1 d .
O26 O -0.14092(18) 0.12720(17) 0.09369(15) 0.0110(4) Uani 1 1 d .
O27 O -0.13229(18) 0.20718(18) -0.05078(16) 0.0123(5) Uani 1 1 d .
O28 O 0.02252(18) 0.01729(17) 0.15803(15) 0.0109(4) Uani 1 1 d .
F1B F 0.44919(17) 0.87512(16) 0.49466(16) 0.0157(5) Uani 0.50 1 d P
O7B O 0.44919(17) 0.87512(16) 0.49466(16) 0.0157(5) Uani 0.50 1 d P
F2 F -0.35592(17) 0.05682(18) 0.04267(16) 0.0242(5) Uani 1 1 d .
C1 C 0.2769(3) 0.5475(3) 0.0668(2) 0.0135(6) Uani 1 1 d .
H1 H 0.2773 0.6074 0.0424 0.016 Uiso 1 1 calc R
C2 C 0.2285(2) 0.4220(2) 0.1341(2) 0.0104(6) Uani 1 1 d .
H2 H 0.1889 0.3787 0.1649 0.013 Uiso 1 1 calc R
C3 C -0.0114(3) 0.8214(2) 0.3460(2) 0.0124(6) Uani 1 1 d .
H3 H -0.0688 0.7882 0.3681 0.015 Uiso 1 1 calc R
C4 C 0.1135(3) 0.8584(2) 0.2635(2) 0.0130(6) Uani 1 1 d .
H4 H 0.1591 0.8560 0.2175 0.016 Uiso 1 1 calc R
C5 C 0.0957(3) 0.5517(2) 0.1280(2) 0.0138(6) Uani 1 1 d .
H5A H 0.0461 0.5016 0.1463 0.017 Uiso 1 1 calc R
H5B H 0.0636 0.5744 0.0734 0.017 Uiso 1 1 calc R
C6 C 0.1169(3) 0.6390(3) 0.2035(2) 0.0148(7) Uani 1 1 d .
H6A H 0.1413 0.6152 0.2600 0.018 Uiso 1 1 calc R
H6B H 0.1722 0.6859 0.1883 0.018 Uiso 1 1 calc R
C7 C 0.0147(3) 0.6902(2) 0.2150(2) 0.0134(6) Uani 1 1 d .
H7A H -0.0179 0.7007 0.1558 0.016 Uiso 1 1 calc R
H7B H -0.0353 0.6479 0.2423 0.016 Uiso 1 1 calc R
C8 C 0.4757(3) 0.3124(2) 0.8595(2) 0.0135(6) Uani 1 1 d .
H8 H 0.4984 0.3482 0.8142 0.016 Uiso 1 1 calc R
C9 C 0.4172(3) 0.1927(3) 0.9300(2) 0.0132(6) Uani 1 1 d .
H9 H 0.3913 0.1303 0.9425 0.016 Uiso 1 1 calc R
C10 C 0.2125(3) -0.0166(3) 0.6230(2) 0.0126(6) Uani 1 1 d .
H10 H 0.1782 -0.0382 0.6709 0.015 Uiso 1 1 calc R
C11 C 0.3349(3) 0.0292(2) 0.5407(2) 0.0107(6) Uani 1 1 d .
H11 H 0.4011 0.0457 0.5210 0.013 Uiso 1 1 calc R
C12 C 0.4267(3) 0.1498(3) 0.7596(2) 0.0157(7) Uani 1 1 d .
H12A H 0.4883 0.1604 0.7261 0.019 Uiso 1 1 calc R
H12B H 0.3643 0.1667 0.7237 0.019 Uiso 1 1 calc R
C13 C 0.4127(3) 0.0418(2) 0.7751(2) 0.0118(6) Uani 1 1 d .
H13A H 0.4728 0.0268 0.8148 0.014 Uiso 1 1 calc R
H13B H 0.3485 0.0309 0.8054 0.014 Uiso 1 1 calc R
C14 C 0.4046(3) -0.0279(3) 0.6871(2) 0.0130(6) Uani 1 1 d .
H14A H 0.4724 -0.0237 0.6610 0.016 Uiso 1 1 calc R
H14B H 0.3898 -0.0958 0.6996 0.016 Uiso 1 1 calc R
C15 C 0.6819(3) 0.4830(3) 0.1554(2) 0.0129(6) Uani 1 1 d .
H15 H 0.7241 0.5355 0.1387 0.015 Uiso 1 1 calc R
C16 C 0.6260(3) 0.3631(3) 0.2254(2) 0.0124(6) Uani 1 1 d .
H16 H 0.6219 0.3166 0.2664 0.015 Uiso 1 1 calc R
C17 C 0.9659(3) 0.2060(3) 0.4317(2) 0.0134(6) Uani 1 1 d .
H17 H 0.9056 0.2138 0.4629 0.016 Uiso 1 1 calc R
C18 C 1.0911(2) 0.2316(2) 0.3462(2) 0.0103(6) Uani 1 1 d .
H18 H 1.1341 0.2601 0.3068 0.012 Uiso 1 1 calc R
C19 C 0.8117(2) 0.4422(2) 0.2814(2) 0.0111(6) Uani 1 1 d .
H19A H 0.8036 0.4862 0.3363 0.013 Uiso 1 1 calc R
H19B H 0.8667 0.4733 0.2498 0.013 Uiso 1 1 calc R
C20 C 0.8465(3) 0.3437(3) 0.3069(2) 0.0135(6) Uani 1 1 d .
H20A H 0.7993 0.3179 0.3484 0.016 Uiso 1 1 calc R
H20B H 0.8437 0.2953 0.2530 0.016 Uiso 1 1 calc R
C21 C 0.9597(3) 0.3616(3) 0.3522(3) 0.0158(7) Uani 1 1 d .
H21A H 1.0051 0.3912 0.3114 0.019 Uiso 1 1 calc R
H21B H 0.9609 0.4086 0.4069 0.019 Uiso 1 1 calc R
O3W O 0.9956(3) 0.6117(3) 0.4102(3) 0.0446(9) Uani 1 1 d .
H3WA H 1.0512 0.5852 0.4285 0.067 Uiso 1 1 d R
H3WB H 0.9430 0.5859 0.4338 0.067 Uiso 1 1 d R
O4W O 0.2349(3) 0.2647(3) 0.6072(3) 0.0491(10) Uani 1 1 d .
O5W O 0.2219(3) 0.2922(3) 0.8624(4) 0.0834(18) Uani 1 1 d .
H5WA H 0.1786 0.3097 0.9010 0.125 Uiso 1 1 d R
H5WB H 0.2191 0.2290 0.8548 0.125 Uiso 1 1 d R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N7 Co1 N7 180.00(14) 2_666 1_554
N7 Co1 N1 89.85(10) 2_666 2_665
N7 Co1 N1 90.15(10) 1_554 2_665
N7 Co1 N1 90.15(10) 2_666 .
N7 Co1 N1 89.85(10) 1_554 .
N1 Co1 N1 180.0 2_665 .
N7 Co1 N13 87.65(10) 2_666 2_665
N7 Co1 N13 92.35(10) 1_554 2_665
N1 Co1 N13 89.84(10) 2_665 2_665
N1 Co1 N13 90.16(10) . 2_665
N7 Co1 N13 92.35(10) 2_666 .
N7 Co1 N13 87.65(10) 1_554 .
N1 Co1 N13 90.16(10) 2_665 .
N1 Co1 N13 89.84(10) . .
N13 Co1 N13 180.00(13) 2_665 .
N7 Co1 Co2 125.70(7) 2_666 .
N7 Co1 Co2 54.30(7) 1_554 .
N1 Co1 Co2 125.77(7) 2_665 .
N1 Co1 Co2 54.23(7) . .
N13 Co1 Co2 126.18(7) 2_665 .
N13 Co1 Co2 53.82(7) . .
N2 Co2 N14 92.23(11) . .
N2 Co2 O16 88.93(10) . .
N14 Co2 O16 177.82(10) . .
N2 Co2 N8 89.24(11) . 1_554
N14 Co2 N8 90.45(11) . 1_554
O16 Co2 N8 87.71(10) . 1_554
N2 Co2 O4 93.59(10) . .
N14 Co2 O4 88.93(10) . .
O16 Co2 O4 92.85(9) . .
N8 Co2 O4 177.12(10) 1_554 .
N2 Co2 O1 173.48(11) . .
N14 Co2 O1 93.57(11) . .
O16 Co2 O1 85.19(10) . .
N8 Co2 O1 87.74(11) 1_554 .
O4 Co2 O1 89.49(10) . .
N2 Co2 Co1 55.08(7) . .
N14 Co2 Co1 55.80(8) . .
O16 Co2 Co1 123.71(7) . .
N8 Co2 Co1 54.69(8) 1_554 .
O4 Co2 Co1 126.86(7) . .
O1 Co2 Co1 126.73(7) . .
N4 Co3 N4 180.0 2_566 1_545
N4 Co3 N10 91.83(10) 2_566 .
N4 Co3 N10 88.17(10) 1_545 .
N4 Co3 N10 88.17(10) 2_566 2_556
N4 Co3 N10 91.83(10) 1_545 2_556
N10 Co3 N10 180.0 . 2_556
N4 Co3 N16 88.95(10) 2_566 1_455
N4 Co3 N16 91.05(10) 1_545 1_455
N10 Co3 N16 91.37(10) . 1_455
N10 Co3 N16 88.63(10) 2_556 1_455
N4 Co3 N16 91.05(10) 2_566 2_656
N4 Co3 N16 88.95(10) 1_545 2_656
N10 Co3 N16 88.63(10) . 2_656
N10 Co3 N16 91.37(10) 2_556 2_656
N16 Co3 N16 180.00(7) 1_455 2_656
N4 Co3 Co4 125.23(7) 2_566 .
N4 Co3 Co4 54.77(7) 1_545 .
N10 Co3 Co4 55.75(7) . .
N10 Co3 Co4 124.25(7) 2_556 .
N16 Co3 Co4 54.19(7) 1_455 .
N16 Co3 Co4 125.81(7) 2_656 .
O3 Co4 O17 88.26(9) . .
O3 Co4 N17 97.19(10) . 1_455
O17 Co4 N17 88.49(10) . 1_455
O3 Co4 N5 171.70(10) . 1_545
O17 Co4 N5 95.31(10) . 1_545
N17 Co4 N5 90.41(11) 1_455 1_545
O3 Co4 N11 86.43(10) . .
O17 Co4 N11 174.31(10) . .
N17 Co4 N11 90.14(11) 1_455 .
N5 Co4 N11 90.22(11) 1_545 .
O3 Co4 O2 86.61(9) . .
O17 Co4 O2 85.00(9) . .
N17 Co4 O2 172.36(10) 1_455 .
N5 Co4 O2 86.23(10) 1_545 .
N11 Co4 O2 96.72(10) . .
O3 Co4 Co3 127.62(7) . .
O17 Co4 Co3 128.98(6) . .
N17 Co4 Co3 56.09(8) 1_455 .
N5 Co4 Co3 54.79(7) 1_545 .
N11 Co4 Co3 53.89(7) . .
O2 Co4 Co3 126.14(6) . .
O4 Mo1 O3 103.47(11) . .
O4 Mo1 O11 100.90(10) . 2_666
O3 Mo1 O11 102.20(10) . 2_666
O4 Mo1 O15 101.85(10) . .
O3 Mo1 O15 91.01(10) . .
O11 Mo1 O15 150.15(10) 2_666 .
O4 Mo1 O14 94.89(10) . .
O3 Mo1 O14 157.03(10) . .
O11 Mo1 O14 87.50(9) 2_666 .
O15 Mo1 O14 71.56(9) . .
O4 Mo1 O12 166.15(10) . 2_666
O3 Mo1 O12 90.23(10) . 2_666
O11 Mo1 O12 73.79(9) 2_666 2_666
O15 Mo1 O12 79.59(9) . 2_666
O14 Mo1 O12 72.34(8) . 2_666
O5 Mo2 O10 104.21(11) . .
O5 Mo2 O12 104.97(11) . .
O10 Mo2 O12 101.37(10) . .
O5 Mo2 O14 102.30(11) . .
O10 Mo2 O14 99.16(10) . .
O12 Mo2 O14 140.36(9) . .
O5 Mo2 O13 96.64(10) . .
O10 Mo2 O13 158.91(10) . .
O12 Mo2 O13 75.82(9) . .
O14 Mo2 O13 72.91(9) . .
O5 Mo2 O14 177.87(10) . 2_666
O10 Mo2 O14 77.69(9) . 2_666
O12 Mo2 O14 75.43(9) . 2_666
O14 Mo2 O14 76.35(9) . 2_666
O13 Mo2 O14 81.41(8) . 2_666
O6 Mo3 F1B 102.33(11) . .
O6 Mo3 O7A 101.88(12) . .
F1B Mo3 O7A 90.88(11) . .
O6 Mo3 O13 98.57(11) . .
F1B Mo3 O13 158.46(9) . .
O7A Mo3 O13 89.88(10) . .
O6 Mo3 O11 92.47(11) . .
F1B Mo3 O11 87.50(10) . .
O7A Mo3 O11 165.58(10) . .
O13 Mo3 O11 86.44(9) . .
O6 Mo3 O12 163.53(11) . .
F1B Mo3 O12 85.20(9) . .
O7A Mo3 O12 92.53(10) . .
O13 Mo3 O12 73.26(9) . .
O11 Mo3 O12 73.05(9) . .
O8 Mo4 O9 103.32(12) . .
O8 Mo4 O15 98.23(11) . .
O9 Mo4 O15 103.79(11) . .
O8 Mo4 O13 97.17(11) . .
O9 Mo4 O13 104.92(11) . .
O15 Mo4 O13 143.13(9) . .
O8 Mo4 O14 102.78(10) . .
O9 Mo4 O14 153.90(11) . .
O15 Mo4 O14 72.16(9) . .
O13 Mo4 O14 71.84(9) . .
O8 Mo4 O10 174.20(10) . 2_666
O9 Mo4 O10 82.44(10) . 2_666
O15 Mo4 O10 80.78(9) . 2_666
O13 Mo4 O10 80.58(9) . 2_666
O14 Mo4 O10 71.46(8) . 2_666
O17 Mo5 O16 101.52(11) . .
O17 Mo5 O23 102.15(10) . .
O16 Mo5 O23 98.79(10) . .
O17 Mo5 O24 103.73(10) . .
O16 Mo5 O24 96.47(10) . .
O23 Mo5 O24 146.53(10) . .
O17 Mo5 O25 153.80(10) . .
O16 Mo5 O25 104.66(10) . .
O23 Mo5 O25 73.05(9) . .
O24 Mo5 O25 74.34(9) . .
O17 Mo5 O28 81.65(9) . .
O16 Mo5 O28 175.61(10) . .
O23 Mo5 O28 83.40(9) . .
O24 Mo5 O28 79.76(9) . .
O25 Mo5 O28 72.25(8) . .
O18 Mo6 O28 104.18(11) . .
O18 Mo6 O26 105.55(11) . .
O28 Mo6 O26 100.74(10) . .
O18 Mo6 O25 103.56(11) . 2
O28 Mo6 O25 97.53(10) . 2
O26 Mo6 O25 140.38(10) . 2
O18 Mo6 O23 99.92(11) . 2
O28 Mo6 O23 155.61(10) . 2
O26 Mo6 O23 75.97(9) . 2
O25 Mo6 O23 73.00(9) 2 2
O18 Mo6 O25 177.91(10) . .
O28 Mo6 O25 73.81(9) . .
O26 Mo6 O25 75.56(8) . .
O25 Mo6 O25 76.28(9) 2 .
O23 Mo6 O25 82.04(8) 2 .
O19 Mo7 O20 105.22(13) . .
O19 Mo7 O27 97.89(12) . .
O20 Mo7 O27 98.42(11) . .
O19 Mo7 F2 90.29(12) . .
O20 Mo7 F2 97.72(11) . .
O27 Mo7 F2 159.28(10) . .
O19 Mo7 O23 163.83(11) . 2
O20 Mo7 O23 88.85(11) . 2
O27 Mo7 O23 87.66(9) . 2
F2 Mo7 O23 79.76(9) . 2
O19 Mo7 O26 97.76(11) . .
O20 Mo7 O26 156.88(10) . .
O27 Mo7 O26 75.53(9) . .
F2 Mo7 O26 84.55(9) . .
O23 Mo7 O26 68.82(8) 2 .
O22 Mo8 O21 103.15(13) . .
O22 Mo8 O27 100.50(11) . .
O21 Mo8 O27 98.12(11) . .
O22 Mo8 O24 97.89(11) . .
O21 Mo8 O24 98.70(11) . .
O27 Mo8 O24 151.47(10) . .
O22 Mo8 O25 163.50(11) . .
O21 Mo8 O25 91.28(10) . .
O27 Mo8 O25 85.08(9) . .
O24 Mo8 O25 71.68(9) . .
O22 Mo8 O26 91.92(10) . .
O21 Mo8 O26 163.81(11) . .
O27 Mo8 O26 72.99(9) . .
O24 Mo8 O26 84.81(9) . .
O25 Mo8 O26 74.74(8) . .
C1 N1 N2 107.0(3) . .
C1 N1 Co1 129.1(2) . .
N2 N1 Co1 123.7(2) . .
C2 N2 N1 107.2(3) . .
C2 N2 Co2 125.8(2) . .
N1 N2 Co2 126.9(2) . .
C2 N3 C1 105.5(3) . .
C2 N3 C5 126.8(3) . .
C1 N3 C5 127.7(3) . .
C3 N4 N5 106.7(3) . .
C3 N4 Co3 128.9(2) . 1_565
N5 N4 Co3 124.3(2) . 1_565
C4 N5 N4 107.5(3) . .
C4 N5 Co4 126.1(2) . 1_565
N4 N5 Co4 126.0(2) . 1_565
C4 N6 C3 105.1(3) . .
C4 N6 C7 126.5(3) . .
C3 N6 C7 128.4(3) . .
C8 N7 N8 107.3(3) . .
C8 N7 Co1 126.7(2) . 1_556
N8 N7 Co1 125.7(2) . 1_556
C9 N8 N7 107.2(3) . .
C9 N8 Co2 127.5(2) . 1_556
N7 N8 Co2 125.2(2) . 1_556
C9 N9 C8 105.5(3) . .
C9 N9 C12 128.8(3) . .
C8 N9 C12 125.5(3) . .
C10 N10 N11 106.7(3) . .
C10 N10 Co3 131.8(2) . .
N11 N10 Co3 121.5(2) . .
C11 N11 N10 107.5(3) . .
C11 N11 Co4 123.2(2) . .
N10 N11 Co4 128.2(2) . .
C11 N12 C10 105.6(3) . .
C11 N12 C14 125.6(3) . .
C10 N12 C14 128.6(3) . .
C15 N13 N14 106.6(3) . .
C15 N13 Co1 128.5(2) . .
N14 N13 Co1 124.8(2) . .
C16 N14 N13 107.3(3) . .
C16 N14 Co2 127.0(2) . .
N13 N14 Co2 125.5(2) . .
C15 N15 C16 105.4(3) . .
C15 N15 C19 126.8(3) . .
C16 N15 C19 127.8(3) . .
C17 N16 N17 106.7(3) . .
C17 N16 Co3 128.1(2) . 1_655
N17 N16 Co3 124.8(2) . 1_655
C18 N17 N16 107.0(2) . .
C18 N17 Co4 128.2(2) . 1_655
N16 N17 Co4 124.8(2) . 1_655
C18 N18 C17 105.6(3) . .
C18 N18 C21 125.6(3) . .
C17 N18 C21 128.8(3) . .
Co4 O2 H2B 110.5 . .
Co4 O2 H2A 110.5 . .
H2B O2 H2A 108.7 . .
Mo1 O3 Co4 147.66(13) . .
Mo1 O4 Co2 160.54(14) . .
Mo2 O10 Mo4 114.87(11) . 2_666
Mo1 O11 Mo3 116.54(11) 2_666 .
Mo2 O12 Mo3 106.43(10) . .
Mo2 O12 Mo1 112.82(11) . 2_666
Mo3 O12 Mo1 93.99(8) . 2_666
Mo4 O13 Mo3 151.54(12) . .
Mo4 O13 Mo2 106.11(10) . .
Mo3 O13 Mo2 101.82(10) . .
Mo2 O14 Mo1 147.64(11) . .
Mo2 O14 Mo4 104.90(9) . .
Mo1 O14 Mo4 95.39(8) . .
Mo2 O14 Mo2 103.65(9) . 2_666
Mo1 O14 Mo2 99.02(8) . 2_666
Mo4 O14 Mo2 95.70(8) . 2_666
Mo4 O15 Mo1 115.11(11) . .
Mo5 O16 Co2 148.28(14) . .
Mo5 O17 Co4 158.97(13) . .
Mo5 O23 Mo6 107.19(10) . 2
Mo5 O23 Mo7 149.82(13) . 2
Mo6 O23 Mo7 102.97(10) 2 2
Mo5 O24 Mo8 115.65(12) . .
Mo6 O25 Mo5 103.27(9) 2 .
Mo6 O25 Mo8 153.08(12) 2 .
Mo5 O25 Mo8 94.82(9) . .
Mo6 O25 Mo6 103.72(9) 2 .
Mo5 O25 Mo6 95.30(8) . .
Mo8 O25 Mo6 94.13(8) . .
Mo6 O26 Mo7 111.08(11) . .
Mo6 O26 Mo8 114.48(10) . .
Mo7 O26 Mo8 91.94(9) . .
Mo7 O27 Mo8 114.38(12) . .
Mo6 O28 Mo5 118.49(11) . .
N1 C1 N3 110.0(3) . .
N1 C1 H1 125.0 . .
N3 C1 H1 125.0 . .
N2 C2 N3 110.4(3) . .
N2 C2 H2 124.8 . .
N3 C2 H2 124.8 . .
N4 C3 N6 110.4(3) . .
N4 C3 H3 124.8 . .
N6 C3 H3 124.8 . .
N5 C4 N6 110.2(3) . .
N5 C4 H4 124.9 . .
N6 C4 H4 124.9 . .
N3 C5 C6 110.2(3) . .
N3 C5 H5A 109.6 . .
C6 C5 H5A 109.6 . .
N3 C5 H5B 109.6 . .
C6 C5 H5B 109.6 . .
H5A C5 H5B 108.1 . .
C7 C6 C5 109.4(3) . .
C7 C6 H6A 109.8 . .
C5 C6 H6A 109.8 . .
C7 C6 H6B 109.8 . .
C5 C6 H6B 109.8 . .
H6A C6 H6B 108.2 . .
N6 C7 C6 110.6(3) . .
N6 C7 H7A 109.5 . .
C6 C7 H7A 109.5 . .
N6 C7 H7B 109.5 . .
C6 C7 H7B 109.5 . .
H7A C7 H7B 108.1 . .
N7 C8 N9 109.9(3) . .
N7 C8 H8 125.1 . .
N9 C8 H8 125.1 . .
N8 C9 N9 110.1(3) . .
N8 C9 H9 124.9 . .
N9 C9 H9 124.9 . .
N10 C10 N12 110.0(3) . .
N10 C10 H10 125.0 . .
N12 C10 H10 125.0 . .
N11 C11 N12 110.1(3) . .
N11 C11 H11 124.9 . .
N12 C11 H11 124.9 . .
N9 C12 C13 110.1(3) . .
N9 C12 H12A 109.6 . .
C13 C12 H12A 109.6 . .
N9 C12 H12B 109.6 . .
C13 C12 H12B 109.6 . .
H12A C12 H12B 108.2 . .
C14 C13 C12 112.1(3) . .
C14 C13 H13A 109.2 . .
C12 C13 H13A 109.2 . .
C14 C13 H13B 109.2 . .
C12 C13 H13B 109.2 . .
H13A C13 H13B 107.9 . .
N12 C14 C13 111.7(3) . .
N12 C14 H14A 109.3 . .
C13 C14 H14A 109.3 . .
N12 C14 H14B 109.3 . .
C13 C14 H14B 109.3 . .
H14A C14 H14B 107.9 . .
N13 C15 N15 110.6(3) . .
N13 C15 H15 124.7 . .
N15 C15 H15 124.7 . .
N14 C16 N15 110.0(3) . .
N14 C16 H16 125.0 . .
N15 C16 H16 125.0 . .
N16 C17 N18 110.5(3) . .
N16 C17 H17 124.7 . .
N18 C17 H17 124.7 . .
N17 C18 N18 110.2(3) . .
N17 C18 H18 124.9 . .
N18 C18 H18 124.9 . .
N15 C19 C20 112.0(3) . .
N15 C19 H19A 109.2 . .
C20 C19 H19A 109.2 . .
N15 C19 H19B 109.2 . .
C20 C19 H19B 109.2 . .
H19A C19 H19B 107.9 . .
C21 C20 C19 108.0(3) . .
C21 C20 H20A 110.1 . .
C19 C20 H20A 110.1 . .
C21 C20 H20B 110.1 . .
C19 C20 H20B 110.1 . .
H20A C20 H20B 108.4 . .
N18 C21 C20 112.3(3) . .
N18 C21 H21A 109.1 . .
C20 C21 H21A 109.1 . .
N18 C21 H21B 109.1 . .
C20 C21 H21B 109.1 . .
H21A C21 H21B 107.9 . .
H3WA O3W H3WB 108.0 . .
H5WA O5W H5WB 108.0 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Co1 N7 2.107(3) 2_666
Co1 N7 2.107(3) 1_554
Co1 N1 2.150(3) 2_665
Co1 N1 2.150(3) .
Co1 N13 2.167(3) 2_665
Co1 N13 2.167(3) .
Co1 Co2 3.8236(4) .
Co2 N2 2.068(3) .
Co2 N14 2.076(3) .
Co2 O16 2.098(2) .
Co2 N8 2.098(3) 1_554
Co2 O4 2.131(2) .
Co2 O1 2.161(3) .
Co3 N4 2.118(3) 2_566
Co3 N4 2.118(3) 1_545
Co3 N10 2.120(3) .
Co3 N10 2.120(3) 2_556
Co3 N16 2.153(3) 1_455
Co3 N16 2.153(3) 2_656
Co3 Co4 3.8028(4) .
Co4 O3 2.055(2) .
Co4 O17 2.061(2) .
Co4 N17 2.076(3) 1_455
Co4 N5 2.092(3) 1_545
Co4 N11 2.097(3) .
Co4 O2 2.154(2) .
Mo1 O4 1.736(2) .
Mo1 O3 1.736(2) .
Mo1 O11 1.836(2) 2_666
Mo1 O15 1.991(2) .
Mo1 O14 2.189(2) .
Mo1 O12 2.355(2) 2_666
Mo2 O5 1.697(2) .
Mo2 O10 1.749(2) .
Mo2 O12 1.875(2) .
Mo2 O14 1.946(2) .
Mo2 O13 2.200(2) .
Mo2 O14 2.451(2) 2_666
Mo3 O6 1.697(2) .
Mo3 F1B 1.822(2) .
Mo3 O7A 1.828(2) .
Mo3 O13 2.010(2) .
Mo3 O11 2.080(2) .
Mo3 O12 2.201(2) .
Mo4 O8 1.701(2) .
Mo4 O9 1.729(2) .
Mo4 O15 1.891(2) .
Mo4 O13 1.955(2) .
Mo4 O14 2.241(2) .
Mo4 O10 2.364(2) 2_666
Mo5 O17 1.735(2) .
Mo5 O16 1.735(2) .
Mo5 O23 1.893(2) .
Mo5 O24 1.910(2) .
Mo5 O25 2.180(2) .
Mo5 O28 2.308(2) .
Mo6 O18 1.704(2) .
Mo6 O28 1.744(2) .
Mo6 O26 1.890(2) .
Mo6 O25 1.953(2) 2
Mo6 O23 2.133(2) 2
Mo6 O25 2.537(2) .
Mo7 O19 1.703(3) .
Mo7 O20 1.721(3) .
Mo7 O27 1.903(2) .
Mo7 F2 1.977(2) .
Mo7 O23 2.189(2) 2
Mo7 O26 2.206(2) .
Mo8 O22 1.710(2) .
Mo8 O21 1.716(2) .
Mo8 O27 1.939(2) .
Mo8 O24 1.953(2) .
Mo8 O25 2.262(2) .
Mo8 O26 2.285(2) .
N1 C1 1.313(4) .
N1 N2 1.384(4) .
N2 C2 1.306(4) .
N3 C2 1.351(4) .
N3 C1 1.355(4) .
N3 C5 1.467(4) .
N4 C3 1.312(4) .
N4 N5 1.375(4) .
N4 Co3 2.118(3) 1_565
N5 C4 1.307(4) .
N5 Co4 2.092(3) 1_565
N6 C4 1.350(4) .
N6 C3 1.353(4) .
N6 C7 1.465(4) .
N7 C8 1.308(4) .
N7 N8 1.382(4) .
N7 Co1 2.107(3) 1_556
N8 C9 1.306(4) .
N8 Co2 2.098(3) 1_556
N9 C9 1.354(4) .
N9 C8 1.357(4) .
N9 C12 1.469(4) .
N10 C10 1.315(4) .
N10 N11 1.380(4) .
N11 C11 1.309(4) .
N12 C11 1.347(4) .
N12 C10 1.357(4) .
N12 C14 1.473(4) .
N13 C15 1.313(4) .
N13 N14 1.378(4) .
N14 C16 1.315(4) .
N15 C15 1.347(4) .
N15 C16 1.348(4) .
N15 C19 1.474(4) .
N16 C17 1.307(4) .
N16 N17 1.386(4) .
N16 Co3 2.153(3) 1_655
N17 C18 1.312(4) .
N17 Co4 2.076(3) 1_655
N18 C18 1.346(4) .
N18 C17 1.348(4) .
N18 C21 1.472(4) .
O2 H2B 0.8500 .
O2 H2A 0.8500 .
O10 Mo4 2.364(2) 2_666
O11 Mo1 1.836(2) 2_666
O12 Mo1 2.355(2) 2_666
O14 Mo2 2.451(2) 2_666
O23 Mo6 2.133(2) 2
O23 Mo7 2.189(2) 2
O25 Mo6 1.953(2) 2
C1 H1 0.9300 .
C2 H2 0.9300 .
C3 H3 0.9300 .
C4 H4 0.9300 .
C5 C6 1.522(5) .
C5 H5A 0.9700 .
C5 H5B 0.9700 .
C6 C7 1.521(4) .
C6 H6A 0.9700 .
C6 H6B 0.9700 .
C7 H7A 0.9700 .
C7 H7B 0.9700 .
C8 H8 0.9300 .
C9 H9 0.9300 .
C10 H10 0.9300 .
C11 H11 0.9300 .
C12 C13 1.511(5) .
C12 H12A 0.9700 .
C12 H12B 0.9700 .
C13 C14 1.511(4) .
C13 H13A 0.9700 .
C13 H13B 0.9700 .
C14 H14A 0.9700 .
C14 H14B 0.9700 .
C15 H15 0.9300 .
C16 H16 0.9300 .
C17 H17 0.9300 .
C18 H18 0.9300 .
C19 C20 1.518(5) .
C19 H19A 0.9700 .
C19 H19B 0.9700 .
C20 C21 1.517(5) .
C20 H20A 0.9700 .
C20 H20B 0.9700 .
C21 H21A 0.9700 .
C21 H21B 0.9700 .
O3W H3WA 0.8500 .
O3W H3WB 0.8500 .
O5W H5WA 0.8501 .
O5W H5WB 0.8500 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
N7 Co1 Co2 N2 60.18(13) 2_666 .
N7 Co1 Co2 N2 -119.82(13) 1_554 .
N1 Co1 Co2 N2 -178.90(13) 2_665 .
N1 Co1 Co2 N2 1.10(13) . .
N13 Co1 Co2 N2 -57.40(13) 2_665 .
N13 Co1 Co2 N2 122.60(13) . .
N7 Co1 Co2 N14 -61.95(13) 2_666 .
N7 Co1 Co2 N14 118.05(13) 1_554 .
N1 Co1 Co2 N14 58.97(13) 2_665 .
N1 Co1 Co2 N14 -121.03(13) . .
N13 Co1 Co2 N14 -179.52(13) 2_665 .
N13 Co1 Co2 N14 0.48(13) . .
N7 Co1 Co2 O16 120.61(12) 2_666 .
N7 Co1 Co2 O16 -59.39(12) 1_554 .
N1 Co1 Co2 O16 -118.46(12) 2_665 .
N1 Co1 Co2 O16 61.54(12) . .
N13 Co1 Co2 O16 3.04(12) 2_665 .
N13 Co1 Co2 O16 -176.96(12) . .
N7 Co1 Co2 N8 178.52(13) 2_666 1_554
N7 Co1 Co2 N8 -1.48(13) 1_554 1_554
N1 Co1 Co2 N8 -60.56(13) 2_665 1_554
N1 Co1 Co2 N8 119.44(13) . 1_554
N13 Co1 Co2 N8 60.95(13) 2_665 1_554
N13 Co1 Co2 N8 -119.05(13) . 1_554
N7 Co1 Co2 O4 -4.48(12) 2_666 .
N7 Co1 Co2 O4 175.52(12) 1_554 .
N1 Co1 Co2 O4 116.44(12) 2_665 .
N1 Co1 Co2 O4 -63.56(12) . .
N13 Co1 Co2 O4 -122.06(12) 2_665 .
N13 Co1 Co2 O4 57.94(12) . .
N7 Co1 Co2 O1 -127.55(14) 2_666 .
N7 Co1 Co2 O1 52.45(14) 1_554 .
N1 Co1 Co2 O1 -6.63(14) 2_665 .
N1 Co1 Co2 O1 173.37(14) . .
N13 Co1 Co2 O1 114.88(14) 2_665 .
N13 Co1 Co2 O1 -65.12(14) . .
N4 Co3 Co4 O3 11.61(12) 2_566 .
N4 Co3 Co4 O3 -168.39(12) 1_545 .
N10 Co3 Co4 O3 -52.69(12) . .
N10 Co3 Co4 O3 127.31(12) 2_556 .
N16 Co3 Co4 O3 69.11(12) 1_455 .
N16 Co3 Co4 O3 -110.89(12) 2_656 .
N4 Co3 Co4 O17 -113.44(13) 2_566 .
N4 Co3 Co4 O17 66.56(13) 1_545 .
N10 Co3 Co4 O17 -177.74(13) . .
N10 Co3 Co4 O17 2.26(13) 2_556 .
N16 Co3 Co4 O17 -55.94(13) 1_455 .
N16 Co3 Co4 O17 124.06(13) 2_656 .
N4 Co3 Co4 N17 -59.25(13) 2_566 1_455
N4 Co3 Co4 N17 120.75(13) 1_545 1_455
N10 Co3 Co4 N17 -123.55(13) . 1_455
N10 Co3 Co4 N17 56.45(13) 2_556 1_455
N16 Co3 Co4 N17 -1.75(13) 1_455 1_455
N16 Co3 Co4 N17 178.25(13) 2_656 1_455
N4 Co3 Co4 N5 -178.26(13) 2_566 1_545
N4 Co3 Co4 N5 1.74(13) 1_545 1_545
N10 Co3 Co4 N5 117.43(13) . 1_545
N10 Co3 Co4 N5 -62.57(13) 2_556 1_545
N16 Co3 Co4 N5 -120.76(13) 1_455 1_545
N16 Co3 Co4 N5 59.24(13) 2_656 1_545
N4 Co3 Co4 N11 60.36(13) 2_566 .
N4 Co3 Co4 N11 -119.64(13) 1_545 .
N10 Co3 Co4 N11 -3.94(13) . .
N10 Co3 Co4 N11 176.06(13) 2_556 .
N16 Co3 Co4 N11 117.86(13) 1_455 .
N16 Co3 Co4 N11 -62.14(13) 2_656 .
N4 Co3 Co4 O2 129.68(12) 2_566 .
N4 Co3 Co4 O2 -50.32(12) 1_545 .
N10 Co3 Co4 O2 65.38(12) . .
N10 Co3 Co4 O2 -114.62(12) 2_556 .
N16 Co3 Co4 O2 -172.82(13) 1_455 .
N16 Co3 Co4 O2 7.18(13) 2_656 .
N7 Co1 N1 C1 48.4(3) 2_666 .
N7 Co1 N1 C1 -131.6(3) 1_554 .
N1 Co1 N1 C1 -139(100) 2_665 .
N13 Co1 N1 C1 -39.3(3) 2_665 .
N13 Co1 N1 C1 140.7(3) . .
Co2 Co1 N1 C1 -175.8(3) . .
N7 Co1 N1 N2 -137.5(3) 2_666 .
N7 Co1 N1 N2 42.5(3) 1_554 .
N1 Co1 N1 N2 35(100) 2_665 .
N13 Co1 N1 N2 134.9(3) 2_665 .
N13 Co1 N1 N2 -45.1(3) . .
Co2 Co1 N1 N2 -1.6(2) . .
C1 N1 N2 C2 0.4(4) . .
Co1 N1 N2 C2 -174.9(2) . .
C1 N1 N2 Co2 178.3(2) . .
Co1 N1 N2 Co2 3.0(4) . .
N14 Co2 N2 C2 -139.7(3) . .
O16 Co2 N2 C2 42.2(3) . .
N8 Co2 N2 C2 129.9(3) 1_554 .
O4 Co2 N2 C2 -50.6(3) . .
O1 Co2 N2 C2 67.5(10) . .
Co1 Co2 N2 C2 175.8(3) . .
N14 Co2 N2 N1 42.8(3) . .
O16 Co2 N2 N1 -135.4(3) . .
N8 Co2 N2 N1 -47.6(3) 1_554 .
O4 Co2 N2 N1 131.8(3) . .
O1 Co2 N2 N1 -110.0(9) . .
Co1 Co2 N2 N1 -1.7(2) . .
C3 N4 N5 C4 0.5(4) . .
Co3 N4 N5 C4 178.0(2) 1_565 .
C3 N4 N5 Co4 -172.7(2) . 1_565
Co3 N4 N5 Co4 4.8(4) 1_565 1_565
C8 N7 N8 C9 -0.8(4) . .
Co1 N7 N8 C9 173.0(2) 1_556 .
C8 N7 N8 Co2 -177.9(2) . 1_556
Co1 N7 N8 Co2 -4.1(4) 1_556 1_556
N4 Co3 N10 C10 54.6(3) 2_566 .
N4 Co3 N10 C10 -125.4(3) 1_545 .
N10 Co3 N10 C10 -110(100) 2_556 .
N16 Co3 N10 C10 143.6(3) 1_455 .
N16 Co3 N10 C10 -36.4(3) 2_656 .
Co4 Co3 N10 C10 -172.8(3) . .
N4 Co3 N10 N11 -126.9(2) 2_566 .
N4 Co3 N10 N11 53.1(2) 1_545 .
N10 Co3 N10 N11 69(100) 2_556 .
N16 Co3 N10 N11 -37.9(2) 1_455 .
N16 Co3 N10 N11 142.1(2) 2_656 .
Co4 Co3 N10 N11 5.68(19) . .
C10 N10 N11 C11 -0.6(4) . .
Co3 N10 N11 C11 -179.4(2) . .
C10 N10 N11 Co4 167.9(2) . .
Co3 N10 N11 Co4 -10.9(4) . .
O3 Co4 N11 C11 -43.3(3) . .
O17 Co4 N11 C11 -64.5(11) . .
N17 Co4 N11 C11 -140.5(3) 1_455 .
N5 Co4 N11 C11 129.1(3) 1_545 .
O2 Co4 N11 C11 42.8(3) . .
Co3 Co4 N11 C11 173.3(3) . .
O3 Co4 N11 N10 149.8(3) . .
O17 Co4 N11 N10 128.6(9) . .
N17 Co4 N11 N10 52.6(3) 1_455 .
N5 Co4 N11 N10 -37.8(3) 1_545 .
O2 Co4 N11 N10 -124.1(3) . .
Co3 Co4 N11 N10 6.4(2) . .
N7 Co1 N13 C15 -50.0(3) 2_666 .
N7 Co1 N13 C15 130.0(3) 1_554 .
N1 Co1 N13 C15 39.8(3) 2_665 .
N1 Co1 N13 C15 -140.2(3) . .
N13 Co1 N13 C15 145(100) 2_665 .
Co2 Co1 N13 C15 176.1(3) . .
N7 Co1 N13 N14 133.2(2) 2_666 .
N7 Co1 N13 N14 -46.8(2) 1_554 .
N1 Co1 N13 N14 -137.0(2) 2_665 .
N1 Co1 N13 N14 43.0(2) . .
N13 Co1 N13 N14 -32(100) 2_665 .
Co2 Co1 N13 N14 -0.7(2) . .
C15 N13 N14 C16 -0.2(4) . .
Co1 N13 N14 C16 177.2(2) . .
C15 N13 N14 Co2 -176.0(2) . .
Co1 N13 N14 Co2 1.3(4) . .
N2 Co2 N14 C16 140.2(3) . .
O16 Co2 N14 C16 -98(3) . .
N8 Co2 N14 C16 -130.5(3) 1_554 .
O4 Co2 N14 C16 46.7(3) . .
O1 Co2 N14 C16 -42.8(3) . .
Co1 Co2 N14 C16 -175.8(3) . .
N2 Co2 N14 N13 -44.8(3) . .
O16 Co2 N14 N13 77(3) . .
N8 Co2 N14 N13 44.5(3) 1_554 .
O4 Co2 N14 N13 -138.3(2) . .
O1 Co2 N14 N13 132.3(2) . .
Co1 Co2 N14 N13 -0.7(2) . .
C17 N16 N17 C18 -0.4(4) . .
Co3 N16 N17 C18 173.1(2) 1_655 .
C17 N16 N17 Co4 -178.3(2) . 1_655
Co3 N16 N17 Co4 -4.8(4) 1_655 1_655
O4 Mo1 O3 Co4 -51.6(3) . .
O11 Mo1 O3 Co4 -156.1(2) 2_666 .
O15 Mo1 O3 Co4 50.9(2) . .
O14 Mo1 O3 Co4 90.6(3) . .
O12 Mo1 O3 Co4 130.5(2) 2_666 .
O17 Co4 O3 Mo1 49.3(2) . .
N17 Co4 O3 Mo1 -38.9(3) 1_455 .
N5 Co4 O3 Mo1 165.0(6) 1_545 .
N11 Co4 O3 Mo1 -128.6(3) . .
O2 Co4 O3 Mo1 134.4(3) . .
Co3 Co4 O3 Mo1 -91.1(2) . .
O3 Mo1 O4 Co2 -82.8(4) . .
O11 Mo1 O4 Co2 22.7(4) 2_666 .
O15 Mo1 O4 Co2 -176.8(4) . .
O14 Mo1 O4 Co2 111.1(4) . .
O12 Mo1 O4 Co2 88.7(6) 2_666 .
N2 Co2 O4 Mo1 -154.1(4) . .
N14 Co2 O4 Mo1 -61.9(4) . .
O16 Co2 O4 Mo1 116.8(4) . .
N8 Co2 O4 Mo1 16(2) 1_554 .
O1 Co2 O4 Mo1 31.7(4) . .
Co1 Co2 O4 Mo1 -106.1(4) . .
O5 Mo2 O10 Mo4 176.70(12) . 2_666
O12 Mo2 O10 Mo4 67.87(13) . 2_666
O14 Mo2 O10 Mo4 -78.03(12) . 2_666
O13 Mo2 O10 Mo4 -12.2(3) . 2_666
O14 Mo2 O10 Mo4 -4.28(10) 2_666 2_666
O6 Mo3 O11 Mo1 -173.21(14) . 2_666
F1B Mo3 O11 Mo1 -70.97(13) . 2_666
O7A Mo3 O11 Mo1 12.9(5) . 2_666
O13 Mo3 O11 Mo1 88.35(13) . 2_666
O12 Mo3 O11 Mo1 14.77(11) . 2_666
O5 Mo2 O12 Mo3 80.98(12) . .
O10 Mo2 O12 Mo3 -170.78(10) . .
O14 Mo2 O12 Mo3 -50.96(19) . .
O13 Mo2 O12 Mo3 -12.23(9) . .
O14 Mo2 O12 Mo3 -96.86(10) 2_666 .
O5 Mo2 O12 Mo1 -177.32(11) . 2_666
O10 Mo2 O12 Mo1 -69.08(12) . 2_666
O14 Mo2 O12 Mo1 50.75(19) . 2_666
O13 Mo2 O12 Mo1 89.48(11) . 2_666
O14 Mo2 O12 Mo1 4.84(9) 2_666 2_666
O6 Mo3 O12 Mo2 75.6(4) . .
F1B Mo3 O12 Mo2 -166.21(12) . .
O7A Mo3 O12 Mo2 -75.53(12) . .
O13 Mo3 O12 Mo2 13.58(10) . .
O11 Mo3 O12 Mo2 104.94(12) . .
O6 Mo3 O12 Mo1 -39.6(4) . 2_666
F1B Mo3 O12 Mo1 78.58(10) . 2_666
O7A Mo3 O12 Mo1 169.25(10) . 2_666
O13 Mo3 O12 Mo1 -101.64(10) . 2_666
O11 Mo3 O12 Mo1 -10.27(8) . 2_666
O8 Mo4 O13 Mo3 82.3(3) . .
O9 Mo4 O13 Mo3 -23.6(3) . .
O15 Mo4 O13 Mo3 -163.6(2) . .
O14 Mo4 O13 Mo3 -176.6(3) . .
O10 Mo4 O13 Mo3 -103.1(3) 2_666 .
O8 Mo4 O13 Mo2 -86.29(12) . .
O9 Mo4 O13 Mo2 167.82(11) . .
O15 Mo4 O13 Mo2 27.8(2) . .
O14 Mo4 O13 Mo2 14.86(9) . .
O10 Mo4 O13 Mo2 88.32(10) 2_666 .
O6 Mo3 O13 Mo4 14.6(3) . .
F1B Mo3 O13 Mo4 -179.5(2) . .
O7A Mo3 O13 Mo4 -87.4(3) . .
O11 Mo3 O13 Mo4 106.5(3) . .
O12 Mo3 O13 Mo4 179.9(3) . .
O6 Mo3 O13 Mo2 -176.63(12) . .
F1B Mo3 O13 Mo2 -10.7(3) . .
O7A Mo3 O13 Mo2 81.38(11) . .
O11 Mo3 O13 Mo2 -84.67(10) . .
O12 Mo3 O13 Mo2 -11.30(9) . .
O5 Mo2 O13 Mo4 83.79(12) . .
O10 Mo2 O13 Mo4 -87.5(3) . .
O12 Mo2 O13 Mo4 -172.39(13) . .
O14 Mo2 O13 Mo4 -17.07(10) . .
O14 Mo2 O13 Mo4 -95.35(10) 2_666 .
O5 Mo2 O13 Mo3 -90.68(12) . .
O10 Mo2 O13 Mo3 98.0(3) . .
O12 Mo2 O13 Mo3 13.14(10) . .
O14 Mo2 O13 Mo3 168.46(12) . .
O14 Mo2 O13 Mo3 90.18(10) 2_666 .
O5 Mo2 O14 Mo1 48.5(2) . .
O10 Mo2 O14 Mo1 -58.4(2) . .
O12 Mo2 O14 Mo1 -178.87(17) . .
O13 Mo2 O14 Mo1 141.7(2) . .
O14 Mo2 O14 Mo1 -133.2(3) 2_666 .
O5 Mo2 O14 Mo4 -78.50(12) . .
O10 Mo2 O14 Mo4 174.66(10) . .
O12 Mo2 O14 Mo4 54.15(18) . .
O13 Mo2 O14 Mo4 14.75(9) . .
O14 Mo2 O14 Mo4 99.81(11) 2_666 .
O5 Mo2 O14 Mo2 -178.31(10) . 2_666
O10 Mo2 O14 Mo2 74.85(10) . 2_666
O12 Mo2 O14 Mo2 -45.67(17) . 2_666
O13 Mo2 O14 Mo2 -85.06(9) . 2_666
O14 Mo2 O14 Mo2 0.0 2_666 2_666
O4 Mo1 O14 Mo2 -44.3(2) . .
O3 Mo1 O14 Mo2 172.5(2) . .
O11 Mo1 O14 Mo2 56.5(2) 2_666 .
O15 Mo1 O14 Mo2 -145.1(2) . .
O12 Mo1 O14 Mo2 130.2(2) 2_666 .
O4 Mo1 O14 Mo4 84.90(10) . .
O3 Mo1 O14 Mo4 -58.3(3) . .
O11 Mo1 O14 Mo4 -174.37(10) 2_666 .
O15 Mo1 O14 Mo4 -15.98(8) . .
O12 Mo1 O14 Mo4 -100.59(9) 2_666 .
O4 Mo1 O14 Mo2 -178.44(9) . 2_666
O3 Mo1 O14 Mo2 38.3(3) . 2_666
O11 Mo1 O14 Mo2 -77.70(9) 2_666 2_666
O15 Mo1 O14 Mo2 80.69(9) . 2_666
O12 Mo1 O14 Mo2 -3.93(7) 2_666 2_666
O8 Mo4 O14 Mo2 76.70(13) . .
O9 Mo4 O14 Mo2 -103.7(2) . .
O15 Mo4 O14 Mo2 171.35(13) . .
O13 Mo4 O14 Mo2 -16.76(10) . .
O10 Mo4 O14 Mo2 -102.64(11) 2_666 .
O8 Mo4 O14 Mo1 -77.87(11) . .
O9 Mo4 O14 Mo1 101.7(2) . .
O15 Mo4 O14 Mo1 16.78(9) . .
O13 Mo4 O14 Mo1 -171.32(11) . .
O10 Mo4 O14 Mo1 102.79(9) 2_666 .
O8 Mo4 O14 Mo2 -177.52(10) . 2_666
O9 Mo4 O14 Mo2 2.1(3) . 2_666
O15 Mo4 O14 Mo2 -82.87(10) . 2_666
O13 Mo4 O14 Mo2 89.02(9) . 2_666
O10 Mo4 O14 Mo2 3.14(7) 2_666 2_666
O8 Mo4 O15 Mo1 80.42(14) . .
O9 Mo4 O15 Mo1 -173.61(13) . .
O13 Mo4 O15 Mo1 -33.3(2) . .
O14 Mo4 O15 Mo1 -20.44(11) . .
O10 Mo4 O15 Mo1 -93.81(12) 2_666 .
O4 Mo1 O15 Mo4 -70.25(14) . .
O3 Mo1 O15 Mo4 -174.24(13) . .
O11 Mo1 O15 Mo4 68.7(2) 2_666 .
O14 Mo1 O15 Mo4 21.01(11) . .
O12 Mo1 O15 Mo4 95.71(13) 2_666 .
O17 Mo5 O16 Co2 -14.9(3) . .
O23 Mo5 O16 Co2 -119.3(3) . .
O24 Mo5 O16 Co2 90.5(3) . .
O25 Mo5 O16 Co2 166.0(2) . .
O28 Mo5 O16 Co2 121.1(12) . .
N2 Co2 O16 Mo5 -110.7(3) . .
N14 Co2 O16 Mo5 127(3) . .
N8 Co2 O16 Mo5 160.0(3) 1_554 .
O4 Co2 O16 Mo5 -17.2(3) . .
O1 Co2 O16 Mo5 72.1(3) . .
Co1 Co2 O16 Mo5 -156.2(2) . .
O16 Mo5 O17 Co4 148.9(4) . .
O23 Mo5 O17 Co4 -109.3(4) . .
O24 Mo5 O17 Co4 49.3(4) . .
O25 Mo5 O17 Co4 -33.1(5) . .
O28 Mo5 O17 Co4 -28.0(4) . .
O3 Co4 O17 Mo5 -136.6(4) . .
N17 Co4 O17 Mo5 -39.3(4) 1_455 .
N5 Co4 O17 Mo5 51.0(4) 1_545 .
N11 Co4 O17 Mo5 -115.4(9) . .
O2 Co4 O17 Mo5 136.7(4) . .
Co3 Co4 O17 Mo5 3.0(4) . .
O17 Mo5 O23 Mo6 167.25(11) . 2
O16 Mo5 O23 Mo6 -88.86(12) . 2
O24 Mo5 O23 Mo6 27.3(2) . 2
O25 Mo5 O23 Mo6 13.88(9) . 2
O28 Mo5 O23 Mo6 87.30(10) . 2
O17 Mo5 O23 Mo7 -10.7(3) . 2
O16 Mo5 O23 Mo7 93.2(3) . 2
O24 Mo5 O23 Mo7 -150.7(2) . 2
O25 Mo5 O23 Mo7 -164.1(3) . 2
O28 Mo5 O23 Mo7 -90.6(2) . 2
O17 Mo5 O24 Mo8 -169.42(12) . .
O16 Mo5 O24 Mo8 87.01(14) . .
O23 Mo5 O24 Mo8 -29.7(2) . .
O25 Mo5 O24 Mo8 -16.45(11) . .
O28 Mo5 O24 Mo8 -90.72(12) . .
O22 Mo8 O24 Mo5 -177.08(13) . .
O21 Mo8 O24 Mo5 -72.39(15) . .
O27 Mo8 O24 Mo5 53.1(3) . .
O25 Mo8 O24 Mo5 16.07(11) . .
O26 Mo8 O24 Mo5 91.69(12) . .
O17 Mo5 O25 Mo6 -97.9(2) . 2
O16 Mo5 O25 Mo6 79.98(12) . 2
O23 Mo5 O25 Mo6 -14.91(10) . 2
O24 Mo5 O25 Mo6 172.71(12) . 2
O28 Mo5 O25 Mo6 -103.27(11) . 2
O17 Mo5 O25 Mo8 102.1(2) . .
O16 Mo5 O25 Mo8 -79.95(10) . .
O23 Mo5 O25 Mo8 -174.84(11) . .
O24 Mo5 O25 Mo8 12.78(9) . .
O28 Mo5 O25 Mo8 96.80(9) . .
O17 Mo5 O25 Mo6 7.5(2) . .
O16 Mo5 O25 Mo6 -174.56(9) . .
O23 Mo5 O25 Mo6 90.55(9) . .
O24 Mo5 O25 Mo6 -81.83(9) . .
O28 Mo5 O25 Mo6 2.19(7) . .
O22 Mo8 O25 Mo6 162.3(3) . 2
O21 Mo8 O25 Mo6 -46.4(3) . 2
O27 Mo8 O25 Mo6 51.6(3) . 2
O24 Mo8 O25 Mo6 -145.1(3) . 2
O26 Mo8 O25 Mo6 125.3(3) . 2
O22 Mo8 O25 Mo5 -65.2(4) . .
O21 Mo8 O25 Mo5 86.06(11) . .
O27 Mo8 O25 Mo5 -175.89(10) . .
O24 Mo8 O25 Mo5 -12.68(9) . .
O26 Mo8 O25 Mo5 -102.20(9) . .
O22 Mo8 O25 Mo6 30.5(4) . .
O21 Mo8 O25 Mo6 -178.26(10) . .
O27 Mo8 O25 Mo6 -80.21(9) . .
O24 Mo8 O25 Mo6 83.01(9) . .
O26 Mo8 O25 Mo6 -6.52(7) . .
O18 Mo6 O25 Mo6 86(3) . 2
O28 Mo6 O25 Mo6 102.19(11) . 2
O26 Mo6 O25 Mo6 -151.84(12) . 2
O25 Mo6 O25 Mo6 0.0 2 2
O23 Mo6 O25 Mo6 -74.35(10) 2 2
O18 Mo6 O25 Mo5 -19(3) . .
O28 Mo6 O25 Mo5 -2.88(9) . .
O26 Mo6 O25 Mo5 103.09(10) . .
O25 Mo6 O25 Mo5 -105.07(11) 2 .
O23 Mo6 O25 Mo5 -179.42(9) 2 .
O18 Mo6 O25 Mo8 -114(3) . .
O28 Mo6 O25 Mo8 -98.11(10) . .
O26 Mo6 O25 Mo8 7.86(9) . .
O25 Mo6 O25 Mo8 159.69(14) 2 .
O23 Mo6 O25 Mo8 85.34(9) 2 .
O18 Mo6 O26 Mo7 -87.93(13) . .
O28 Mo6 O26 Mo7 163.92(11) . .
O25 Mo6 O26 Mo7 47.93(19) 2 .
O23 Mo6 O26 Mo7 8.67(10) 2 .
O25 Mo6 O26 Mo7 93.91(11) . .
O18 Mo6 O26 Mo8 169.64(12) . .
O28 Mo6 O26 Mo8 61.48(13) . .
O25 Mo6 O26 Mo8 -54.50(19) 2 .
O23 Mo6 O26 Mo8 -93.76(12) 2 .
O25 Mo6 O26 Mo8 -8.53(9) . .
O19 Mo7 O26 Mo6 161.87(13) . .
O20 Mo7 O26 Mo6 -24.6(3) . .
O27 Mo7 O26 Mo6 -101.93(12) . .
F2 Mo7 O26 Mo6 72.32(12) . .
O23 Mo7 O26 Mo6 -8.79(10) 2 .
O19 Mo7 O26 Mo8 -80.91(11) . .
O20 Mo7 O26 Mo8 92.6(3) . .
O27 Mo7 O26 Mo8 15.29(8) . .
F2 Mo7 O26 Mo8 -170.46(9) . .
O23 Mo7 O26 Mo8 108.43(9) 2 .
O22 Mo8 O26 Mo6 -160.54(13) . .
O21 Mo8 O26 Mo6 40.6(4) . .
O27 Mo8 O26 Mo6 99.06(13) . .
O24 Mo8 O26 Mo6 -62.79(12) . .
O25 Mo8 O26 Mo6 9.61(11) . .
O22 Mo8 O26 Mo7 85.20(10) . .
O21 Mo8 O26 Mo7 -73.6(4) . .
O27 Mo8 O26 Mo7 -15.20(8) . .
O24 Mo8 O26 Mo7 -177.05(9) . .
O25 Mo8 O26 Mo7 -104.65(9) . .
O19 Mo7 O27 Mo8 76.08(14) . .
O20 Mo7 O27 Mo8 -177.15(13) . .
F2 Mo7 O27 Mo8 -36.3(4) . .
O23 Mo7 O27 Mo8 -88.67(12) 2 .
O26 Mo7 O27 Mo8 -19.94(11) . .
O22 Mo8 O27 Mo7 -69.32(15) . .
O21 Mo8 O27 Mo7 -174.41(13) . .
O24 Mo8 O27 Mo7 60.0(2) . .
O25 Mo8 O27 Mo7 95.00(12) . .
O26 Mo8 O27 Mo7 19.47(11) . .
O18 Mo6 O28 Mo5 -177.52(12) . .
O26 Mo6 O28 Mo5 -68.30(13) . .
O25 Mo6 O28 Mo5 76.38(13) 2 .
O23 Mo6 O28 Mo5 11.4(3) 2 .
O25 Mo6 O28 Mo5 3.08(10) . .
O17 Mo5 O28 Mo6 178.76(15) . .
O16 Mo5 O28 Mo6 42.2(13) . .
O23 Mo5 O28 Mo6 -77.88(14) . .
O24 Mo5 O28 Mo6 73.08(14) . .
O25 Mo5 O28 Mo6 -3.61(12) . .
N2 N1 C1 N3 -0.5(4) . .
Co1 N1 C1 N3 174.4(2) . .
C2 N3 C1 N1 0.5(4) . .
C5 N3 C1 N1 177.5(3) . .
N1 N2 C2 N3 -0.1(4) . .
Co2 N2 C2 N3 -178.1(2) . .
C1 N3 C2 N2 -0.2(4) . .
C5 N3 C2 N2 -177.3(3) . .
N5 N4 C3 N6 0.7(4) . .
Co3 N4 C3 N6 -176.7(2) 1_565 .
C4 N6 C3 N4 -1.5(4) . .
C7 N6 C3 N4 177.9(3) . .
N4 N5 C4 N6 -1.4(4) . .
Co4 N5 C4 N6 171.8(2) 1_565 .
C3 N6 C4 N5 1.8(4) . .
C7 N6 C4 N5 -177.6(3) . .
C2 N3 C5 C6 104.4(4) . .
C1 N3 C5 C6 -72.0(4) . .
N3 C5 C6 C7 173.7(3) . .
C4 N6 C7 C6 49.5(5) . .
C3 N6 C7 C6 -129.8(4) . .
C5 C6 C7 N6 -167.9(3) . .
N8 N7 C8 N9 0.8(4) . .
Co1 N7 C8 N9 -172.9(2) 1_556 .
C9 N9 C8 N7 -0.4(4) . .
C12 N9 C8 N7 175.2(3) . .
N7 N8 C9 N9 0.5(4) . .
Co2 N8 C9 N9 177.5(2) 1_556 .
C8 N9 C9 N8 -0.1(4) . .
C12 N9 C9 N8 -175.5(3) . .
N11 N10 C10 N12 -0.1(4) . .
Co3 N10 C10 N12 178.5(2) . .
C11 N12 C10 N10 0.7(4) . .
C14 N12 C10 N10 -173.6(3) . .
N10 N11 C11 N12 1.1(4) . .
Co4 N11 C11 N12 -168.1(2) . .
C10 N12 C11 N11 -1.1(4) . .
C14 N12 C11 N11 173.4(3) . .
C9 N9 C12 C13 -18.5(5) . .
C8 N9 C12 C13 166.9(3) . .
N9 C12 C13 C14 -176.2(3) . .
C11 N12 C14 C13 115.1(3) . .
C10 N12 C14 C13 -71.6(4) . .
C12 C13 C14 N12 -54.3(4) . .
N14 N13 C15 N15 1.0(4) . .
Co1 N13 C15 N15 -176.2(2) . .
C16 N15 C15 N13 -1.4(4) . .
C19 N15 C15 N13 179.3(3) . .
N13 N14 C16 N15 -0.6(4) . .
Co2 N14 C16 N15 175.1(2) . .
C15 N15 C16 N14 1.2(4) . .
C19 N15 C16 N14 -179.4(3) . .
N17 N16 C17 N18 0.7(4) . .
Co3 N16 C17 N18 -172.5(2) 1_655 .
C18 N18 C17 N16 -0.8(4) . .
C21 N18 C17 N16 -179.9(3) . .
N16 N17 C18 N18 -0.1(4) . .
Co4 N17 C18 N18 177.8(2) 1_655 .
C17 N18 C18 N17 0.5(4) . .
C21 N18 C18 N17 179.7(3) . .
C15 N15 C19 C20 -145.8(3) . .
C16 N15 C19 C20 35.0(4) . .
N15 C19 C20 C21 169.9(3) . .
C18 N18 C21 C20 121.1(4) . .
C17 N18 C21 C20 -59.9(5) . .
C19 C20 C21 N18 -177.5(3) . .
